Transformation from slip to plastic flow deformation ... Transformation from slip to plastic flow...
Embed Size (px)
Transcript of Transformation from slip to plastic flow deformation ... Transformation from slip to plastic flow...
Transformation from slip to plastic flow deformation mechanism during tensile deformation of zirconium nanocontacts
著者 Yamada Kohei, Kizuka Tokushi journal or publication title
volume 7 page range 42901 year 2017-02 権利 (C) The Author(s) 2017
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
URL http://hdl.handle.net/2241/00145625 doi: 10.1038/srep42901
Creative Commons : 表示 http://creativecommons.org/licenses/by/3.0/deed.ja
1Scientific RepoRts | 7:42901 | DOI: 10.1038/srep42901
Transformation from slip to plastic flow deformation mechanism during tensile deformation of zirconium nanocontacts Kohei Yamada & Tokushi Kizuka
Various types of nanometer-sized structures have been applied to advanced functional and structural devices. Inherent structures, thermal stability, and properties of such nanostructures are emphasized when their size is decreased to several nanometers, especially, to several atoms. In this study, we observed the atomistic tensile deformation process of zirconium nanocontacts, which are typical nanostructures used in connection of nanometer-sized wires, transistors, and diodes, memory devices, and sensors, by in situ transmission electron microscopy. It was found that the contact was deformed via a plastic flow mechanism, which differs from the slip on lattice planes frequently observed in metals, and that the crystallinity became disordered. The various irregular relaxed structures formed during the deformation process affected the conductance.
As the size of metals decreases to the nanometer scale, dislocation motion is suppressed, or even absent, while applying external forces. When the grain size of polycrystalline metals is decreased to 10–100 nm, grain bound- ary sliding and grain rotation govern deformation instead of dislocation-mediated slip1–7. In particular, as the width of deformation region is reduced to several atoms, the deformation mechanism is transformed from dislocation-mediated slip to non-slip manners, i.e., homogeneous slip8–12. After the transformation of deforma- tion mechanics, the critical shear stress of nanometer-size metals increases by several tens of times or more in comparison with that of dislocation-mediated slip, e.g., ~1 GPa for silver11 (Ag) and ~5 GPa for rhodium12 (Rh). Such a transformation is observed in metallic nanocontacts (NCs) with face-centered cubic (fcc) structures10–12. Since the number of primary slip systems in fcc structure metals is 12, slip along equivalent slip systems can occur easily13; deformation via slip continues until the size is reduced to less than several nanometers and subsequent fracture occurs, regardless of whether the dislocation is mediated. Conversely, the primary slip system of metals with hexagonal-closed packed (hcp) structure is limited to only three equivalent systems on basal planes13. In addition, the rotation of the deformation regions of NCs is suppressed since the region is fixed by two adjacent rigid tips11. Atomic-size contacts of zinc (Zn) with an hcp structure show unstable melting-like behavior, related to different break conductance features from NCs of other metals14. Theoretical treatments, such as molecular dynamics (MD) simulations, show that the atomic configuration of the deformation region becomes disordered during the deformation in NCs with width less than several atoms; the deformation proceeds while the crystal structure crumbles and all atoms in the deformation region move simultaneously in a way like atomic motion in liquid9,15–26. Thus, atomistic observation of the deformation process of hcp-structure metal NCs is expected to reveal new deformation mechanics. In this paper, we focus on zirconium (Zr) NCs with this goal in mind.
Results Figure 1 shows the time series of high-resolution transmission electron microscopy (TEM) images of the tensile deformation process of a Zr NC (Supplementary Movie 1). Both the upper and lower dark regions in each image correspond to the Zr nanotips. The regions around the NC correspond to vacuum. The two types of lattice fringes observed on both nanotips correspond to the (0002) and (1011) planes with hcp-structure Zr spacing of 0.26 nm and 0.25 nm, respectively. The incident-electron-beam direction, i.e., the observation direction of the NC, is par- allel to the  direction. From the lattice fringes it is found that the NC is a tilt grain boundary with a rotation
Division of Materials Science, Faculty of Pure and Applied Sciences, University of Tsukuba, Tsukuba, Ibaraki 305- 8573, Japan. Correspondence and requests for materials should be addressed to T.K. (email: firstname.lastname@example.org. ac.jp)
received: 05 March 2016
accepted: 17 January 2017
Published: 20 February 2017
2Scientific RepoRts | 7:42901 | DOI: 10.1038/srep42901
angle of 90 ± 1°. First, the NC with a 5-atom-wide minimum cross section is shown in Fig. 1(a) and (b). When a tensile force acts on the NC, the upper nanotip slides on the (0001) plane of the lower nanotip, as indicated by the arrow in Fig. 1(a). Thus, slip occurs along the boundary plane. This slip corresponds to the typical slip system on the basal plane of an hcp structure [Fig. 1(a)–(e)]. Figure 2 shows the time series of the enlarged high-resolution images of the slip region in Fig. 1(a)–(e) and the models of their atomic configuration. The direction of the tensile force (the bold arrows in Fig. 2) is parallel to the upper direction, whereas the slip direction (the fine arrows in Fig. 2) is parallel to the (0001) basal plane of the lower nanotip, which tilts from the tensile direction. Thus, the slip direction tilts away from the tensile force direction. This deformation causes a decrease in contact width of five atoms [Fig. 2(c)], four atoms [Fig. 2(d)], three atoms [Fig. 2(e)], and two atoms [Fig. 2(f)]. Subsequently, the upper nanotip moves along the tensile force direction, i.e., the direction approximately perpendicular to the slip plane. Figure 3 shows the time series of the enlarged high-resolution images of the deformation region from Fig. 1(f ) and the models of their atomic configuration (The time of Fig. 1(f ) is defined as 0 s for easy-to-understand). The constriction region (the shaded regions in Fig. 3) expands along the direction parallel to the direction of tensile force (the bold arrows in Fig. 3). By this expansion, the interatomic distance in the deformation region is elongated and the bond angles become different from that inside the nanotips; the atomic configuration in the deformation region crumbles from the hcp unit cell. Thus, we found clearly that this defor- mation is non-slip deformation. Note that although the two types of lattice fringes observed clearly on both nanotips beside the minimum cross section, the lattice image of this region became blurred (see Supplementary Movie 1), indicating that the structure in the deformation region becomes disordered. Since stress does not become concentrated on a certain atomic plane during this deformation, atoms in the contact regions show dif- fusive motion similar to that in liquids although the contact is solid. Hence, we found that the deformation in NCs
Figure 1. Time series of high-resolution images of Zr NC tensile deformation. The NC was elongated along the direction indicated by the arrow in Fig. 1a. The minimum cross-sectional width for each image is five atoms [(a), (b)], four atoms [(c)], three atoms [(d), (e)], two atoms [(f), (g)], and one atom [(h)]. (i) shows fracture. (See Supplementary Movie 1.) The average strain rate was 1.4 × 10−2/s.
3Scientific RepoRts | 7:42901 | DOI: 10.1038/srep42901
proceeds in a plastic flow manner. During the deformation, the contact width decreases from two atoms [Fig. 1(g)] to one atom [Fig. 1(h)]. The contact eventually fractures [Fig. 1(i)]. The observation reveals that, as the contact width decreases, the deformation mechanism transforms from slip on lattice planes to plastic flow deformation.
Figure 4 shows the variations in minimum cross-sectional width and conductance of the Zr NC during the tensile deformation process presented in Fig. 1 as a function of time. As the minimum cross-sectional width decreases, the conductance also decreases. The conductance increases rapidly at time g, as shown in Fig. 4. A similar increase in conductance is also observed between times h and i before contact fracture.
Figure 5 shows the histogram of time-conductance traces obtained during the tensile deformation processes of Zr NCs. The number of accumulated traces was 90. In the histogram, broad peaks are observed at 0.5G0 (G0 = 2e2/h, where e is the electron charge and h is Planck’s constant) and 1.8G0. These peaks do not correspond to the positions of integral multiples of G0. Thus, the features of the conductance quantization are not observed27–34.
Figure 6 shows the ratio of the number of plateaus at each conductance value to all observed plateaus. We defined the plateaus as the duration of the p